#------------------------------------------------------------------------------
#$Date: 2019-11-23 18:01:24 +0100 (Sat 23 de Nov de 2019) $
#$Revision: 234556 $
#$URL: svn://www.crystallography.net/cod/cif/7/12/51/7125149.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7125149
loop_
_publ_author_name
'Lekin, Kristina'
'Ogata, Kazuma'
'Maclean, Adrian'
'Mailman, Aaron'
'Winter, Stephen M.'
'Assoud, Abdeljalil'
'Mito, Masaki'
'Tse, John S.'
'Desgreniers, Serge'
'Hirao, Naohisa'
'Dube, Paul A.'
'Oakley, Richard T.'
_publ_section_title
;
 Pushing TC to 27.5 K in a heavy atom radical ferromagnet.
;
_journal_issue                   96
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              13877
_journal_page_last               13880
_journal_paper_doi               10.1039/c6cc07142b
_journal_volume                  52
_journal_year                    2016
_chemical_formula_moiety         'C7 H5 I1 N3 Se4'
_chemical_formula_sum            'C7 H5 I N3 Se4'
_chemical_formula_weight         573.88
_chemical_melting_point_gt       400
_chemical_name_common            IBPSSEt
_chemical_name_systematic
; 
8-iodo-4-ethyl-4H-bis[1,2,3]diselenazolo[4,5-b:5',4'-e]pyridin-2-yl
;
_space_group_IT_number           113
_space_group_name_Hall           'P -4 2ab'
_space_group_name_H-M_alt        'P -4 21 m'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'P -4 2ab'
_symmetry_space_group_name_H-M   'P -4 21 m'
_audit_creation_date             2016-08-29T13:34
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2016-08-29T13:34  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   15.9014(14)
_cell_length_b                   15.9014
_cell_length_c                   3.7840(24)
_cell_measurement_temperature    293(2)
_cell_volume                     956.8(6)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device_type  'SPring-8 BL10XU'
_diffrn_radiation_polarisn_ratio 0.95
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.41358
_diffrn_source                   Synchrotron
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.986
_pd_block_id
2016-08-29T13:34|IBPSSET_496GPA_DONE2|Oakley|SPring-8
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_phase_name
'from C:/gsas/MyWork/IBPSSEt/4.96GPa/4.96 GPa_RT.cif'
_pd_proc_info_datetime           2016-08-29T13:34:38
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with  8 terms.
 Shifted Chebyshev function of 1st kind
      1:    2471.27     2:    1134.56     3:   -121.553     4:   -2.76500    
      5:    59.7430     6:   -6.04778     7:   -22.1398     8:   0.735835    
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =  679.367 #2(GV)   =  -27.662 #3(GW)   =    0.881
 #4(LX)   =    1.721 #5(LY)   =   64.195 #6(trns) =   -6.074
 #7(asym) =  -0.0415 #8(shft) =  -0.1415 #9(GP)   =    0.345
 #10(stec)=   331.89 #11(ptec)=     5.12 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.012 #18(L23) =   -0.023
 Peak tails are ignored  where the intensity is below 0.0010 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0409
_pd_proc_ls_prof_wR_expected     0.0183
_pd_proc_ls_prof_wR_factor       0.0534
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   2.91
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.26072
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.02
_reflns_d_resolution_high        1.661
_reflns_d_resolution_low         7.951
_reflns_limit_h_max              13
_reflns_limit_h_min              0
_reflns_limit_k_max              9
_reflns_limit_k_min              0
_reflns_limit_l_max              3
_reflns_limit_l_min              0
_reflns_number_total             89
_cod_data_source_file            c6cc07142b4.cif
_cod_data_source_block           1c_5_0_GPa
_cod_depositor_comments
;
The following automatic conversions were performed:

data name '_chemical_melting_point' was changed to
'_chemical_melting_point_gt' since the value was specified as 'more
than' ('>') a certain temperature.

data item '_geom_angle_publ_flag' value 'N' was changed to 'n' in
accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26 (18 times).

data item '_geom_bond_publ_flag' value 'N' was changed to 'n' in
accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26 (13 times).

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        956.8(5)
_cod_database_code               7125149
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 +y,-x,-z
3 -x,-y,+z
4 -y,+x,-z
5 -x+1/2,+y+1/2,-z
6 +y+1/2,+x+1/2,+z
7 +x+1/2,-y+1/2,-z
8 -y+1/2,-x+1/2,+z
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
I I1 -0.93068 -0.56933 -0.79162 1.0 Uiso 0.0777 4
N N2 -0.7529 -0.74711 -1.51451 1.0 Uiso 0.0777 4
C C3 -0.85159 -0.64842 -1.07661 1.0 Uiso 0.0777 4
C C4 -0.70207 -0.79794 -1.75947 1.0 Uiso 0.0777 4
C C5 -0.64225 -0.85776 -1.58279 1.0 Uiso 0.0777 4
H H5A -0.61035 -0.88966 -1.75632 1.0 Uiso 0.1554 4
Se Se1 -0.60248 -0.55201 -1.31133 1.0 Uiso 0.0777 8
Se Se2 -0.7292 -0.51506 -1.02808 1.0 Uiso 0.0777 8
N N1 -0.64148 -0.65113 -1.47672 1.0 Uiso 0.0777 8
C C1 -0.71823 -0.6719 -1.38786 1.0 Uiso 0.0777 8
C C2 -0.77219 -0.61944 -1.17496 1.0 Uiso 0.0777 8
H H4A -0.66991 -0.75977 -1.90712 1.0 Uiso 0.1554 8
H H5B -0.60466 -0.82532 -1.43474 1.0 Uiso 0.1554 8
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
I 4.0 0.000 0.000 20.1472 4.34700 18.9949 0.38140 7.51380 27.7660 2.27350
66.8776 4.07120 International_Tables_Vol_C
N 12.0 0.000 0.000 12.2126 0.00570 3.13220 9.89330 2.01250 28.9975 1.16630
0.58260 -11.529 International_Tables_Vol_C
C 28.0 0.000 0.000 2.31000 20.8439 1.02000 10.2075 1.58860 0.56870 0.86500
51.6512 0.21560 International_Tables_Vol_C
H 20.0 0.000 0.000 0.49300 10.5109 0.32291 26.1257 0.14019 3.14236 0.04081
57.7997 0.00304 International_Tables_Vol_C
Se 16.0 0.000 0.000 17.0006 2.40980 5.81960 0.27260 3.97310 15.2372 4.35430
43.8163 2.84090 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
I1 I1 C3 148.770 3_345 1_555 n
C4 N2 C1 117.907 1_555 1_555 n
I1 C3 C2 119.075 1_555 1_555 n
N2 C4 C5 114.534 1_555 1_555 n
N2 C4 H4A 107.968 1_555 1_555 n
C5 C4 H4A 108.574 1_555 1_555 n
C4 C5 H5A 111.104 1_555 1_555 n
C4 C5 H5B 108.126 1_555 1_555 n
H5A C5 H5B 110.279 1_555 1_555 n
Se2 Se1 N1 94.680 1_555 1_555 n
Se1 Se2 C2 87.496 1_555 1_555 n
Se1 N1 C1 116.850 1_555 1_555 n
N2 C1 N1 119.638 1_555 1_555 n
N2 C1 C2 116.774 1_555 1_555 n
N1 C1 C2 123.5316 1_555 1_555 n
C3 C2 Se2 122.839 1_555 1_555 n
C3 C2 C1 119.763 1_555 1_555 n
Se2 C2 C1 117.358 1_555 1_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
I1 C3 2.0800 1_555 n
N2 C4 1.4717 1_555 n
N2 C1 1.40139 1_555 n
C4 C5 1.50220 1_555 n
C4 H4A 0.97060 1_555 n
C5 H5A 0.97252 1_555 n
C5 H4A 2.0316 1_555 n
Se1 Se2 2.35677 1_555 n
Se1 N1 1.80569 1_555 n
Se2 C2 1.87913 1_555 n
N1 C1 1.30828 1_555 n
C1 C2 1.44261 1_555 n
C2 C3 1.39461 1_555 n
